Commenced in January 2007
Paper Count: 30172
Effect of Polymer Molecular Structures on Properties of Dental Cement Restoratives
Abstract:The objective of this study was to synthesize and characterize the poly(alkenoic acid)s with different molecular structures, use these polymers to formulate a dental cement restorative, and study the effect of molecular structures on reaction kinetics, viscosity, and mechanical strengths of the formed polymers and cement restoratives. In this study, poly(alkenoic acid)s with different molecular structures were synthesized. The purified polymers were formulated with commercial Fuji II LC glass fillers to form the experimental cement restoratives. The reaction kinetics was studied via 1HNMR spectroscopy. The formed restoratives were evaluated using compressive strength, diametral tensile strength, flexural strength, hardness and wear-resistance tests. Specimens were conditioned in distilled water at 37oC for 24 h prior to testing. Fuji II LC restorative was used as control. The results show that the higher the arm number and initiator concentration, the faster the reaction was. It was also found that the higher the arm number and branching that the polymer had, the lower the viscosity of the polymer in water and the lower the mechanical strengths of the formed restorative. The experimental restoratives were 31-53% in compressive strength, 37- 55% in compressive modulus, 80-126% in diametral tensile strength, 76-94% in flexural strength, 4-21% in fracture toughness and 53-96% in hardness higher than Fuji II LC. For wear test, the experimental restoratives were only 5.4-13% of abrasive and 6.4-12% of attritional wear depths of Fuji II LC in each wear cycle. The aging study also showed that all the experimental restoratives increased their strength continuously during 30 days, unlike Fuji II LC. It is concluded that polymer molecular structures have significant and positive impact on mechanical properties of dental cement restoratives.
Digital Object Identifier (DOI): doi.org/10.5281/zenodo.1109918Procedia APA BibTeX Chicago EndNote Harvard JSON MLA RIS XML ISO 690 PDF Downloads 1127
 D. C. Smith, “Development of Glass-ionomer Cement Systems,” Biomaterials, Vol. 9, pp. 467-478, 1998.
 A. D. Wilson and J. W. McLean, “Glass-ionomer Cements,” Quintessence Publ Co., Chicago, 1988.
 C. L. Davidson and I. A. Mjör, “Advances in Glass-ionomer Cements,” Quintessence Publ Co., Chicago, 1999.
 A. D. Wilson, “Resin-modified Glass-ionomer Cement,” The International journal of prosthodontics, Vol. 3, pp. 425-429, 1990.
 P. Hotz, J. W. McLean, I. Sced and A. D. Wilson, “The Bonding of Glass-ionomer Cements to Metal and Tooth Substrates,” British Dental Journal, Vol. 142, pp. 41-47, 1977.
 W. R. Lacefield, M. C. Reindl and D. H. Retief, “Tensile Bond Strength of A Glass-ionomer Cement,” The Journal of Prosthetic Dentistry, Vol. 53, pp. 194-198, 1985.
 L. Forsten, “Fluoride Release from A Glass-ionomer Cement,” Scandinavian Journal of Dental Research, Vol. 85, pp. 503-504, 1977.
 R. G. Craig, “Restorative Dental Materials,” 10th Edition, Mosby-Year Book, Inc St Louis, 1997.
 J. W. Nicholson, J. H. Braybrook and E. A. Wasson, “The Biocompatibility of Glass-poly(alkenoate) Glass-ionomer Cements: A Review,” Journal of Biomaterials Science. Polymer Edition, Vol. 2, pp. 277-285, 1991.
 W. R. Hume and G. J. Mount, “In Vitro Studies on the Potential for Pulpal Cytotoxicity of Glass-ionomer Cements. Journal of Dental Research,” Vol. 67, 915-918, 1988.
 R. Guggenberger, R. May and K. P. Stefan, “New Trends in Glassionomer Chemistry,” Biomaterials, Vol. 19, pp. 479-483, 1998.
 S. B. Mitra, Adhesion to Dentin and Physical Properties of A Lightcured Glass-ionomer Liner/Base,” Journal of Dental Research, Vol. 70, pp. 72-74, 1991.
 Y. Momoi, K. Hirosaki, A. Kohno and J. F. McCabe, “Flexural Properties of Resin-modified Hybrid Glass-ionomers in Comparison with Conventional Acid-base Glass-ionomers,” Dental Materials Journal, Vol. 14, pp. 109-119, 1995.
 D. Xie, B. M. Culbertson and W. M. Johnston, “Formulations of Lightcurable Glass-ionomer Cements Containing N-Vinylpyrrolidone,” Journal of Macromolecular Science, Part A Pure and Applied Chemistry, Vol. A35, pp. 1631-1650, 1998.
 D. Xie, W. Wu, A. Puckett, B. Farmer and J. Mays, “Novel Resinmodified Glass-ionomer Cements with Improved Flexural Strength and Ease of Handling,” European Polymer Journal, Vol. 40, pp. 343-351, 2004.
 E. C. Kao, B. M. Culbertson and D. Xie, “Preparation of Glass-ionomer Cement Using N-Acryloyl-Substituted Amino Acid Monomers: Evaluation of Physical Properties,” Dental Materials, Vol. 12, pp. 44-51, 1996.
 D. Xie, I. D. Chung, W. Wu, J. Lemons, A. Puckett and J. Mays, “An Amino Acid Modified and Non-HEMA Containing Glass-ionomer Cement,” Biomaterials, Vol. 25, pp. 1825-1830, 2004.
 D. Xie, B. M. Culbertson and W. M. Johnston, “Improved Flexural Strength of N-Vinylpyrrolidone Modified Acrylic Acid Copolymers for Glass-ionomers,” Journal of Macromolecular Science, Part A Pure and Applied Chemistry, Vol. A35, pp. 1615-1629, 1998.
 P. Bahadur and N. V. Sastry, “Principles of Polymer Science,” CRC press, Boca Raton, 2002.
 C. F. Huang, H. F. Lee, S. W. Kuo, H. Xu and F. C. Chang, “Star Polymers via Atom Transfer Radical Polymerization from Adamantinebased Cores,” Polymer, Vol. 45, pp. 2261-2269, 2004.
 D. Xie, J. G. Park and J. Zhao, “Synthesis and Preparation of Novel 4- Arm Star-shape Poly(carboxylic acid)s for Improved Light-cured Glassionomer Cements,” Dental Materials, Vol. 23, pp. 395-403, 2007.
 D. Xie, Y. Yang, J. Zhao, J. G. Park and J. T. Zhang, “A Novel Comonomer-free Light-cured Glass-ionomer Cement for Reduced Cytotoxicity and Enhanced Mechanical Strength,” Dental Materials, Vol. 23, p. 994-1003, 2007.
 J. Zhao and D. Xie, “A Novel Hyperbranched Poly(acrylic acid) for Improved Resin-modified Glass-ionomer Restoratives,” Dental Materials, Vol. 27, pp. 478-486, 2011.
 W. W. Johnson, V. B. Dhuru and W. A. Brantley, “Composite Microfiller Content and Its Effect on Fracture Toughness and Diametral Tensile Strength,” Dental Materials, Vol. 9, pp. 95-98, 1993.
 D. Xie, W. A. Brantley, B. M. Culbertson and G. Wang, “Mechanical Properties and Microstructures of Glass-ionomer Cements,” Dental Materials, Vol. 16, p. 129-138, 2000.
 A. H. Dowling and G. J. P. Fleming, “The Impact of Montmorillonite Clay Addition on the In Vitro Wear Resistance of A Glass-ionomer Restorative,” Journal of Dentistry, Vol. 35, pp. 309-317, 2007.
 J. R. Condon and J. L. Ferracane, “Evaluation of Composite Wear with A New Multi-Mode Oral Wear Simulator,” Dental Materials, Vol. 12, pp. 218-226, 1996.
 C. P. Turssi, J. L. Ferracane and K. Vogel, “Filler Features and Their Effects on Wear and Degree of Conversion of Particulate Dental Resin Composites,” Biomaterials, Vol. 26, pp. 4932-4937, 2005.
 K. Matyjaszewski and J. Xia, “Atom Transfer Radical Polymerization,” Chemical Reviews, Vol. 101, pp. 2921-2990, 2001.
 D. A. Shipp and K. Matyjaszewski, “Kinetic Analysis of Controlled/“Living” Radical Polymerizations by Simulations. 1. The Importance of Diffusion-controlled Reactions,” Macromolecules, Vol. 32, pp. 2948, 1999.
 D. A. Shipp and K. Matyjaszewski, “Kinetic Analysis of Controlled/“Living” Radical Polymerizations by Simulations. 2. Apparent External Orders of Reactants in Atom Transfer Radical Polymerization,” Macromolecules, Vol. 33, pp. 1553-1559, 2000.
 M. A. Cattani-Lorente, C. Godin and J. M. Meyer, “Mechanical Behavior of Glass ionomer Cements Affected by Long-term Storage in Water,” Dental Materials, Vol. 10, pp. 37-44, 1994.
 G. J. Pearson and A. S. Atkinson, “Long-term Flexural Strength of Glass-ionomer Cements,” Biomaterials, Vol. 12, pp. 658-660, 1991.